Statement of problem
Despite the expanded applications for zirconia in restorative dentistry, there is no clear recommendation in the literature regarding surface treatment before bonding.
The purpose of this study was to evaluate the effect of mechanical surface treatment of yttria-partially stabilized zirconia on its flexural strength and the effect of mechanical and chemical surface treatments on its bond strength to a resin cement.
Material and methods
For flexural strength evaluation, zirconia bars (4 × 5 × 40 mm) were prepared from zirconia blocks, finished using a diamond rotary cutting instrument, sintered, then assigned into 4 groups: (1) control (no treatment), (2) airborne-particle abrasion, (3) silicoating, and (4) wet hand grinding. After storage for 24 hours at 37°C, flexural strength was determined using a 3-point bending test, and the results were analyzed using 1-way ANOVA (α=.05). For shear bond strength evaluation, zirconia rods (2.5 × 3 mm) were prepared from zirconia blocks, sintered, and assigned into 16 groups. Each group underwent a combination of the following mechanical and chemical treatments. Mechanical treatment included: (1) control (no treatment), (2) airborne-particle abrasion, (3) silicoating, or (4) wet hand grinding. Chemical treatment included: (1) control (no treatment), (2) acid etching followed by silanation, (3) silanation only, or (4) application of zirconia primer. Dentin specimens were prepared from extracted molars stored in 0.5% chloramine-T. Zirconia rods were bonded to dentin using a resin cement (Multilink Automix), then light polymerized. After storage, the specimens were loaded to failure with the notched shear bond test method in a universal loading apparatus. For artificial aging analysis, the groups that achieved the highest bond strength values were duplicated, stored at 37°C and 100% humidity for 90 days, and thermal cycled before being loaded to failure. Results were analyzed using 2-way ANOVA (α=.05).
Airborne-particle abrasion and hand grinding significantly increased flexural strength. The highest shear bond strength values were achieved for the following groups: silicoated + silanated > hand ground + zirconia primer > airborne-particle abraded + silanated > zirconia primer > airborne-particle abraded + zirconia primer. Artificial aging resulted in significantly lower shear bond strength for the silicoated/silanated and the zirconia primer groups.
Mechanical modification of the surface increased the flexural strength of Y-TZP. The resin bond to Y-TZP was improved by surface treatment. A combination of mechanical and chemical conditioning of the zirconia surface was essential to develop a durable resin bond to zirconia. (J Prosthet Dent 2010;103:210-220)
To read this article in full you will need to make a payment
Purchase one-time access:Academic & Personal: 24 hour online accessCorporate R&D Professionals: 24 hour online access
One-time access price info
- For academic or personal research use, select 'Academic and Personal'
- For corporate R&D use, select 'Corporate R&D Professionals'
Subscribe:Subscribe to Journal of Prosthetic Dentistry
Already a print subscriber? Claim online access
Already an online subscriber? Sign in
Register: Create an account
Institutional Access: Sign in to ScienceDirect
- Perspective on the development of high-toughness ceramics.J Am Ceram Soc. 1990; 73: 187-206
- Microtensile bond strength of different components of core veneered all-ceramic restorations.Dent Mater. 2005; 21: 984-991
- Contemporary all-ceramic fixed partial dentures: a review.Dent Clin North Am. 2004; 48: 531-544
- Fracture resistance of human enamel and three all-ceramic crown systems on extracted teeth.Int J Prosthodont. 1996; 9: 580-585
- Marginal adaptation and microleakage of Procera AllCeram crowns with four cements.Int J Prosthodont. 2004; 17: 529-535
- Long-term clinical success of all-ceramic posterior restorations.Quintessence Int. 2002; 3: 415-426
- A comparison of the microstructure and properties of the IPS Empress 2 and the IPS Empress glass-ceramics.J Biomed Mater Res. 2000; 53: 297-303
- Long-term resin bond strength to zirconia ceramic.J Adhes Dent. 2000; 2: 139-147
- Effect of etching and airborne particle abrasion on the microstructure of different dental ceramics.J Prosthet Dent. 2003; 89: 479-488
- Strengthening by surface damage in metastable tetragonal zirconia.J Am Ceram Soc. 1980; 63: 117
- A technique for introducing surface compression into zirconia ceramics.J Am Ceram Soc. 1983; 66: c178-c179
- Effect of grinding on strength of tetragonal zirconia and zirconia-toughened alumina.Mach Sci Technol. 1997; 1: 49-66
- Strength and reliability of surface treated Y-TZP dental ceramics. J.Biomed Mater Res. 2000; 53: 304-313
- Effect of silica coating and silanization on flexural and composite-resin bond strengths of zirconia posts: an in vitro study.J Prosthet Dent. 2006; 95: 224-229
- The effect of surface grinding and sandblasting on flexural strength and reliability of Y-TZP zirconia ceramic.Dent Mater. 1999; 15: 426-433
- Sandblasting and silica coating of a glass infiltrated alumina ceramic: volume loss, morphology, and changes in the surface composition.J Prosthet Dent. 1994; 71: 453-461
- Damage accumulation and fatigue life of particle-abraded ceramics.Int J Prosthodont. 2006; 19: 442-448
- Effect of sandblasting on the long-term performance of dental ceramics.J Biomed Mater Res B Appl Biomater. 2004; 71: 381-386
- Influence of surface and heat treatments on the flexural strength of Y-TZP dental ceramic.J Dent. 2005; 33: 9-18
- Metastablility of the martensitic transformation in a 12 mol% ceria-zirconia alloy: II, grinding studies.J Am Ceram Soc. 1989; 72: 1358-1364
- Effect of surface conditioning methods on the bond strength of luting cement to ceramics.Dent Mater. 2003; 19: 725-731
- Bonding to zirconia ceramic: adhesion methods and their durability.Dent Mater. 1998; 14: 64-71
- Bond strength of composite luting cement to zirconia ceramic surfaces.Dent Mater. 2005; 21: 1158-1162
- The influence of ceramic surface treatments on the tensile bond strength of composite resin to all-ceramic coping materials.J Prosthet Dent. 2005; 94: 357-362
- Influence of surface treatment and simulated aging on bond strengths of luting agents to zirconia.Quintessence Int. 2007; 38: 745-753
- The effect of silica coating on the resin bond to the intaglio surface of Procera AllCeram restorations.Quintessence Int. 2003; 34: 542-547
- In vitro evaluation of shear bond strengths of resin to densly-sintered high-purity zirconium-oxide ceramic after long-term storage and thermal cycling.J Prosthet Dent. 2004; 91: 356-362
- Selective infiltration-etching technique for a strong and durable bond of resin cements to zirconia-based materials.J Prosthet Dent. 2007; 98: 379-388
- ANSI/ADA Specification No. 69. Dental ceramic: 1999. American Dental Association, Chicago1999
- Bond strength of luting cements to zirconium oxide ceramics.Int J Prosthodont. 2000; 13: 131-135
- Influence of post-etching cleaning and connecting porcelain on the microtensile bond strength of composite resin to feldspathic porcelain.J Prosthet Dent. 2006; 96: 354-361
- Thermal cycling procedures for laboratory testing of dental restorations.J Dent. 1999; 27: 89-99
- In vivo measurements of thermal diffusion through restorations of various materials.J Prosthet Dent. 1980; 43: 180-185
- Microle akage: the effect of storage and cycling duration.J Prosthet Dent. 1987; 57: 574-576
- Hydrolytic stability of self-etch adhesives bonded to dentin.J Dent Res. 2005; 84: 1160-1164
- ISO TR 11405:1994. Dental materials-guidance on testing of adhesion to tooth structure. ISO, Geneva1994
Supported by the American Academy of Fixed Prosthodontics Tylman Research Grant Program (2006), and second-place recipient of the Tylman research award (2009).
Presented as a poster presentation at the American Academy of Fixed Prosthodontics annual meeting, Chicago, Ill, Feb 2008, and Feb 2009.
© 2010 The Editorial Council of the Journal of Prosthetic Dentistry. Published by Elsevier Inc. All rights reserved.